Used as semiconductor material for a-Si solar cells, or thin-film silicon solar cells, it is deposited in thin films onto a variety of flexible substrates, such as glass, metal and plastic. Amorphous silicon cells generally feature low efficiency, but are one of the most environmentally friendly photovoltaic technologies, since they do not use any toxic heavy metals such as cadmium or lead.
As a second-generation thin-film solar cell technology, amorphous silicon was once expected to become a major contributor in the fast-growing worldwide photovoltaic market, but has since lost its significance due to strong competition from conventional crystalline silicon cells and other thin-film technologies such as CdTe and CIGS.
- 1 Description
- 2 Amorphous silicon and carbon
- 3 Deposition processes
- 4 Applications
- 5 See also
- 6 References
- 7 External links
- 8 Further reading
Silicon is a fourfold coordinated atom that is normally tetrahedrally bonded to four neighboring silicon atoms. In crystalline silicon (c-Si) this tetrahedral structure continues over a large range, thus forming a well-ordered crystal lattice.
In amorphous silicon this long range order is not present. Rather, the atoms form a continuous random network. Moreover, not all the atoms within amorphous silicon are fourfold coordinated. Due to the disordered nature of the material some atoms have a dangling bond. Physically, these dangling bonds represent defects in the continuous random network and may cause anomalous electrical behavior.
The material can be passivated by hydrogen, which bonds to the dangling bonds and can reduce the dangling bond density by several orders of magnitude. Hydrogenated amorphous silicon (a-Si:H) has a sufficiently low amount of defects to be used within devices such as solar photovoltaic cells, particularly in the protocrystalline growth regime. However, hydrogenation is associated with light-induced degradation of the material, termed the Staebler–Wronski effect.
Amorphous silicon and carbon
Amorphous alloys of silicon and carbon (amorphous silicon carbide, also hydrogenated, a-Si1-xCx:H) are an interesting variant. Introduction of carbon atoms adds extra degrees of freedom for control of the properties of the material. The film could also be made transparent to visible light.
Increasing concentrations of carbon in the alloy widen the electronic gap between conduction and valence bands (also called "optical gap" and bandgap). This can potentially increase the light efficiency of solar cells made with amorphous silicon carbide layers. On the other hand, the electronic properties as a semiconductor (mainly electron mobility), are adversely affected by the increasing content of carbon in the alloy, due to the increased disorder in the atomic network.
Several studies are found in the scientific literature, mainly investigating the effects of deposition parameters on electronic quality, but practical applications of amorphous silicon carbide in commercial devices are still lacking.
|Type of film||a-Si:H||a-Si:H||a-Si:H||a-Si|
|Unique application||Large-area electronics||Hydrogen-free deposition|
|Active element temperature||2000C|
|Chamber pressure||0.1-10 Torr||0.1-10 Torr||0.001-0.1 Torr|
|Physical principle||Thermolysis||Plasma-induced dissociation||Thermolysis||Ionization of Si source|
|Facilitators||W/Ta heated wires||Argon cations|
|Typical drive voltage||RF 13.56 MHz; 0.01-1W/cm2|
|Si source||SiH4 gas||SiH4 gas||SiH4 gas||crusible|
While a-Si suffers from lower electronic performance compared to c-Si, it is much more flexible in its applications. For example, a-Si layers can be made thinner than c-Si, which may produce savings on silicon material cost.
One further advantage is that a-Si can be deposited at very low temperatures, e.g., as low as 75 degrees Celsius. This allows for deposition on not only glass, but plastic as well, making it a candidate for a roll-to-roll processing technique. Once deposited, a-Si can be doped in a fashion similar to c-Si, to form p-type or n-type layers and ultimately to form electronic devices.
Another advantage is that a-Si can be deposited over large areas by PECVD. The design of the PECVD system has great impact on the production cost of such panel, therefore most equipment suppliers put their focus on the design of PECVD for higher throughput, that leads to lower manufacturing cost particularly when the silane is recycled.
Amorphous silicon (a-Si) has been used as a photovoltaic solar cell material for devices which require very little power, such as pocket calculators, because their lower performance compared to conventional crystalline silicon (c-Si) solar cells is more than offset by their simplified and lower cost of deposition onto a substrate. The first solar powered calculators were already available in the late 1970s, such as the Royal Solar 1, Sharp EL-8026, and Teal Photon.
More recently, improvements in a-Si construction techniques have made them more attractive for large-area solar cell use as well. Here their lower inherent efficiency is made up, at least partially, by their thinness – higher efficiencies can be reached by stacking several thin-film cells on top of each other, each one tuned to work well at a specific frequency of light. This approach is not applicable to c-Si cells, which are thick as a result of their construction technique and are therefore largely opaque, blocking light from reaching other layers in a stack.
The main advantage of a-Si in large scale production is not efficiency, but cost. a-Si cells use only a fraction of the silicon needed for typical c-Si cells, and the cost of the silicon has historically been a significant contributor to cell cost. However, the higher costs of manufacture due to the multi-layer construction have, to date, made a-Si unattractive except in roles where their thinness or flexibility are an advantage.
Typically, amorphous silicon thin-film cells use a p-i-n structure. Typical panel structure includes front side glass, TCO, thin-film silicon, back contact, polyvinyl butyral (PVB) and back side glass. Uni-Solar, a division of Energy Conversion Devices produced a version of flexible backings, used in roll-on roofing products. However, the world's largest manufacturer of amorphous silicon photovoltaics had to file for bankruptcy in 2012, as it could not compete with the rapidly declining prices of conventional solar panels.
Microcrystalline and micromorphous silicon
- Microcrystalline silicon (also called nanocrystalline silicon) is amorphous silicon, but also contains small crystals. It absorbs a broader spectrum of light and is flexible. Micromorphous silicon module technology combines two different types of silicon, amorphous and microcrystalline silicon, in a top and a bottom photovoltaic cell. Sharp produces cells using this system in order to more efficiently capture blue light, increasing the efficiency of the cells during the time where there is no direct sunlight falling on them. Protocrystalline silicon is often used to optimize the open circuit voltage of a-Si photovoltaics.
- Xunlight Corporation, which has received over $40 million of institutional investments, has completed the installation of its first 25 MW wide-web, roll-to-roll photovoltaic manufacturing equipment for the production of thin-film silicon PV modules. Anwell Technologies has also completed the installation of its first 40 MW a-Si thin film solar panel manufacturing facility in Henan with its in-house designed multi-substrate-multi-chamber PECVD equipment.
Photovoltaic thermal hybrid solar collectors
- Photovoltaic thermal hybrid solar collectors (PVT), are systems that convert solar radiation into thermal and electrical energy. These systems combine a solar cell, which converts electromagnetic radiation (photons) into electricity, with a solar thermal collector, which captures the remaining energy and removes waste heat from the solar PV module. Solar cells suffer from a drop in efficiency with the rise in temperature due to increased resistance. Most such systems can be engineered to carry heat away from the solar cells thereby cooling the cells and thus improving their efficiency by lowering resistance. Although this is an effective method, it causes the thermal component to under-perform compared to a solar thermal collector. Recent research showed that a-Si:H PV with low temperature coefficients allow the PVT to be operated at high temperatures, creating a more symbiotic PVT system and improving performance of the a-Si:H PV by about 10%.
Thin-film-transistor liquid-crystal display
Amorphous silicon has become the material of choice for the active layer in thin-film transistors (TFTs), which are most widely used in large-area electronics applications, mainly for liquid-crystal displays (LCDs).
Thin-film-transistor liquid-crystal display (TFT-LCD) show a similar circuit layout process to that of semiconductor products. However, rather than fabricating the transistors from silicon, that is formed into a crystalline silicon wafer, they are made from a thin film of amorphous silicon that is deposited on a glass panel. The silicon layer for TFT-LCDs is typically deposited using the PECVD process. Transistors take up only a small fraction of the area of each pixel and the rest of the silicon film is etched away to allow light to easily pass through it.
Polycrystalline silicon is sometimes used in displays requiring higher TFT performance. Examples include small high-resolution displays such as those found in projectors or viewfinders. Amorphous silicon-based TFTs are by far the most common, due to their lower production cost, whereas polycrystalline silicon TFTs are more costly and much more difficult to produce.
- R.W. Collins, et al., "Evolution of microstructure and phase in amorphous, protocrystalline, and microcrystalline silicon studied by real time spectroscopic ellipsometry", Solar Energy Materials and Solar Cells, 78(1-4), pp. 143-180, 2003.
- S. Y. Myong, S. W. Kwon, J. H. Kwak, K. S. Lim, J. M. Pearce, and M. Konagai, "Good stability of protocrystalline silicon multilayer solar cells against light irradiation originating from vertically regular distribution of isolated nano-sized silicon grains", 4th World Conference on Photovoltaic Energy Conversion Proceedings, p. 492, 2006.
- C. R. Wronski, et al., "Intrinsic and Light Induced Gap States in a-Si:H Materials and Solar Cells - Effects of Microstructure", Thin Solid Films, 451-452 pp. 470-475, 2004.
- "Towards very low-cost mass production of thin-film silicon photovoltaic (PV) solar modules on glass". Elsevier B.V. 2005-09-02.
- M. A. Kreiger, et al., Life Cycle Analysis of Silane Recycling in Amorphous Silicon-Based Solar Photovoltaic Manufacturing, Resources, Conservation & Recycling, 70, pp.44-49 (2013). http://www.academia.edu/2310926/Life_Cycle_Analysis_of_Silane_Recycling_in_Amorphous_Silicon-Based_Solar_Photovoltaic_Manufacturing
- "The End Arrives for ECD Solar". GreentechMedia. 14 February 2012.
- "Oerlikon Divests Its Solar Business and the Fate of Amorphous Silicon PV". GrrentechMedia. March 2, 2012.
- Pearce, J. M.; Podraza, N.; Collins, R. W.; Al-Jassim, M. M.; Jones, K. M.; Deng, J.; Wronski, C. R. (June 2007). "Optimization of open circuit voltage in amorphous silicon solar cells with mixed-phase (amorphous+nanocrystalline) p-type contacts of low nanocrystalline content" (PDF). Journal of Applied Physics 101 (11): 114301 — 114301–7. doi:10.1063/1.2714507.
- "Xunlight Completes Installation of its First 25 Megawatt Wide-Web Roll-to-Roll Photovoltaic Manufacturing Equipment". Xunlight. June 22, 2009.
- "Anwell Produces its First Thin Film Solar Panel". Solarbuzz. September 7, 2009.
- S.A. Kalogirou, Y. Tripanagnostopoulos (30 January 2006). These systems are most often used for domestic hot water (DHW) and electricity production
- Pathak, M. J. M.; Pearce, J. M.; Harrison, S. J. (2012). "Effects on amorphous silicon photovoltaic performance from high-temperature annealing pulses in photovoltaic thermal hybrid devices". Solar Energy Materials and Solar Cells 100: 199–203. arXiv:1203.1216. doi:10.1016/j.solmat.2012.01.015.
- "TFT LCD - Fabricating TFT LCD". Plasma.com. Retrieved 2013-07-21.
- "TFT LCD - Electronic Aspects of LCD TVs and LCD Monitors". Plasma.com. Retrieved 2013-07-21.
- Amorphous Silicon Devices group at the University of Waterloo, Ontario, Canada
- Theory and Simulation at Ohio University, Athens Ohio